3 Alternating hybrid algorithms: CNT growth by MD/fbMC
Tải bản đầy đủ - 0trang
Theor Chem Acc (2013) 132:1320
state. The red atoms indicate the carbon atoms involved in the
formation of the new diamond 6-ring. Reproduced from [74] with
permission from the Royal Society of Chemistry
Fig. 3 Formation of a new diamond 6-ring from an adsorbed C-atom
and adsorbed C2H2 molecule as observed in a MD/MMC simulation.
a The initial conﬁguration, b–d intermediate states and e the ﬁnal
and electronic properties. However, these properties are
directly determined by their precise structure, thus necessitating very accurate control over the growth process. In
this case, atomistic simulations may provide the atomic
scale insight needed to understand how the growth process
might be controlled, and why speciﬁc structures are formed
for a given growth condition.
One very important factor during the growth is the phase
state of the nanocatalyst. Thus, we performed MD/fbMC
simulations, employing the Shibuta potential, to determine
the phase state of various Ni-nanoparticles as a function of
size and temperature [76]. In this work, the thermalization
was carried out using combined MD/fbMC simulations.
Analysis of the radial distribution of the atomic Lindemann
index revealed that that for the smallest clusters, a dynamic
coexistence process occurs. As illustrated in Fig. 4, surface
melting is observed for the larger particles. In all cases, a
signiﬁcant depression of the melting temperature relative to
the bulk was observed, due to the Gibbs–Thomson effect,
in agreement with the literature [77–79].
Subsequently, a number of combined MD/fbMC simulations were performed to study the growth of carbon
nanotubes based on the ReaxFF potential to gain an
atomic scale understanding in the actual growth process
[80–82]. In these simulations, rather conservative values
for D=2 ¼ 0:085Req [80] and D=2 ¼ 0:07Req [81, 82] in
the fbMC were chosen. The temperature was set to 1,000 K,
corresponding to a typical experimental growth temperature. After each MC cycle, new random velocities were
assigned to all atoms, and the simulation was continued
with constant temperature MD. Similar to Grein et al., the
impact and deposition of atoms (in this case C-atoms) on
the substrate (in this case a Ni-nanocluster) were followed
by MD, and the subsequent relaxation by fbMC. It was
found that the fbMC method results in healing of the carbon network that is formed by the continuous addition of
carbon atoms—a process in which high barriers must be
overcome. An example of this healing mechanism as
Reprinted from the journal
Fig. 4 Calculated radial distribution of the atomic Lindemann index
for a Ni244 cluster, for various temperatures, revealing a surface
melting mechanism. Reproduced from [15] with permission from the
American Chemical Society
observed in the fbMC is shown in Fig. 5. This then ﬁnally
leads to CNTs with very few defects, as illustrated in
Fig. 6, in contrast to what is typically observed in pure MD
growth simulations. Both metallic tubes [81] as well as
semi-conducting tubes [80] could be obtained. Furthermore, we also observed that the chirality of the tube may
change in the initial nucleation stage. It was found that this
is due to the incorporation of asymmetric defects, such as
so-called 5–7 defects [81]. Thus, these MD/fbMC simulations allow to gain an understanding of how the longer
timescale events may inﬂuence the growth process.
In another study, we used MD/fbMC simulations to
investigate how an electric ﬁeld may inﬂuence the growth
process. In agreement with the experiment [83, 84], SWNT
285
123
Theor Chem Acc (2013) 132:1320
simulations directly provide information about the relevant
processes complementary to the experiment.
5 Conclusion
In this contribution, we have presented a brief summary of
the main accelerated molecular dynamics techniques as
well as more a elaborate description of the various techniques for combining MD simulations with MC simulations, as an alternative to accelerated molecular dynamics
simulations for generating long system trajectories. Using
examples from the literature, it is shown that combined
MD/MC simulations may provide a dynamic picture of a
reactive system, including relaxation events which take
place on timescales typically beyond the reach of pure MD.
Essentially, we can distinguish between algorithms in
which some atoms are moved by MD and some by MC
(combined MD/MC method), algorithms in which the
atomic displacement prescription is in part deterministic
and in part stochastic (hybrid MD/MC method), and algorithm in which MD cycles alternate with MC cycles
(sequential MD/MC method).
Three representative examples from our own research
efforts were shown to demonstrate the applicability of MD/
MC simulations, viz. Cu adatom diffusion, UNCD growth
and CNT growth.
In addition to their ease of implementation and their
general applicability make these methods very attractive
for studying systems in which processes beyond the reach
of standard MD are important.
Fig. 5 Observed healing mechanism of the growing carbon network
during CNT growth. Reproduced from [81] with the permission of the
American Chemical Society
Fig. 6 Simulated SWNT
growth based on the MD/fbMC
technique, resulting in a SWNT
with (7, 7) chirality.
Reproduced from [81] with
permission from the American
Chemical Society
References
1. Frenkel D, Smit B (2001) Understanding molecular simulation:
from algorithms to applications. Academic Press, London
2. Cooke DJ, Elliott JA (2007) Atomistic simulations of calcite
nanoparticles and their interaction with water. J Chem Phys
127(10). Art no 104706
3. Khalilov U, Pourtois G, van Duin ACT, Neyts EC (2012) selflimiting oxidation in small-diameter Si nanowires. Chem Mater
24(11):2141–2147
4. Lu Y, Cheng H, Chen M (2012) A molecular dynamics examination of the relationship between self-diffusion and viscosity in
liquid metals. J Chem Phys 136(21). Art no 214505
5. Matsukuma M, Hamaguchi S (2008) Molecular dynamics simulation of microcrystalline Si deposition processes by silane
plasmas. Thin Solid Films 516(11):3443–3448
6. Neyts E, Bogaerts A, Gijbels R, Benedikt J, Van De Sanden M
(2004) Molecular dynamics simulations for the growth of diamond-like carbon ﬁlms from low kinetic energy species. Diam
Relat Mater13(10):1873–1881
7. Faccioli P, Lonardi A, Orland H (2010) Dominant reaction
pathways in protein folding: a direct validation against molecular
dynamics simulations. J Chem Phys 133(4). Art no 045104
Fig. 7 MD/fbMC simulation of vertically aligned SWNT growth by
applying an electric ﬁeld of 700 kV/cm [82]
alignment was observed if a (sufﬁciently strong) electric
ﬁeld was applied. This is shown in Fig. 7 for an electric
ﬁeld value of 700 kV/cm. These simulations shed a new
light on the underlying mechanism: we found that the
electric ﬁeld is primarily acting on the polar Ni–C bonds, at
the interface between the nickel nanocluster and the
growing SWNT. Thus, as at this interface the C-atoms are
slightly negative, while the Ni-atoms are slightly positive,
the carbon atoms experience both an oriented force, pulling
them toward the tip of the cluster, but are also subject to
random thermal diffusion. If the electric ﬁeld is sufﬁciently
strong, the directed migration dominates the random diffusion, an a vertically aligned SWNT emerges. Thus, these
123
286
Reprinted from the journal
Theor Chem Acc (2013) 132:1320
8. Rauf S, Sparks T, Ventzek PLG, Smirnov VV, Stengach AV,
Gaynullin KG, Pavlovsky VA (2007) A molecular dynamics
investigation of ﬂuorocarbon based layer-by-layer etching of
silicon and SiO2. J Appl Phys 101(3). Art no 033308
9. Gou F, Neyts E, Eckert M, Tinck S, Bogaerts A (2010) Molecular
dynamics simulations of Cl? etching on a Si(100) surface. J Appl
Phys 107(11):113305
10. Postawa Z, Czerwinski B, Szewczyk M, Smiley E, Winograd N,
Garrison B (2003) Enhancement of sputtering yields due to C-60
versus Ga bombardment of Ag{111} as explored by molecular
dynamics simulations. Anal Chem 75(17):4402–4407
11. Shen XJ, Xiao Y, Dong W, Yan XH, Busnengo HF (2012)
Molecular dynamics simulations based on reactive force-ﬁelds for
surface chemical reactions. Comput Theor Chem 990: 152–158
12. Servantie J, Gaspard P (2003) Methods of calculation of a friction
coefﬁcient: application to nanotubes. Phys Rev Lett 91(18). Art
no 185503
13. Thaulow C, Sen D, Buehler MJ (2011) Atomistic study of the
effect of crack tip ledges on the nucleation of dislocations in
silicon single crystals at elevated temperature. Mater Sci Eng A
Struct Mater Prop Microstruct Process 528(13–14):4357–4364
14. Shibuta Y (2012) Phase transition of metal nanowires conﬁned in
a low-dimensional nanospace. Chem Phys Lett 532:84–89
15. Neyts EC, Bogaerts A (2009) Numerical study of the sizedependent melting mechanisms of nickel nanoclusters. J Phys
Chem C 113(7):2771–2776
16. Dongare AM, Rajendran AM, LaMattina B, Zikry MA, Brenner
DW (2009) Atomic scale studies of spall behavior in nanocrystalline Cu. J Appl Phys 108(11):113518
17. Shaw DE, Maragakis P, Lindorff-Larsen K, Piana S, Dror RO,
Eastwood MP, Bank JA, Jumper JM, Salmon JK, Shan Y,
Wriggers W (2010) Atomic-level characterization of the structural dynamics of proteins. Science 330(6002):341–346
18. Metropolis N, Rosenbluth AW, Rosenbluth MN, Teller AH,
Teller E (1953) Equation of state calculations by fast computing
machines. J Chem Phys 21(6):1087
19. Kikuchi K, Yoshida M, Maekawa T, Watanabe H (1991)
Metropolis Monte–Carlo method as a numerical technique to solve
the Fokker-Planck equation. Chem Phys Lett 185(3–4): 335–338
20. Kikuchi K, Yoshida M, Maekawa T, Watanabe H (1992)
Metropolis Monte-Carlo method for Brownian dynamics simulation generalized to include hydrodynamic interactions. Chem
Phys Lett 196(1–2):57–61
21. Bortz AB, Kalos MH, Leibowitz JL (1975) A new algorithm for
Monte Carlo simulation of Ising spin systems. J Comput Phys
17:10–18
22. Netto A, Frenklach M (2005) Kinetic Monte Carlo simulations of
CVD diamond growth—interlay among growth, etching, and
migration. Diam Relat Mater 14(10):1630–1646
23. Henkelman G, Jonsson H (2001) Long time scale kinetic Monte
Carlo simulations without lattice approximation and predeﬁned
event table. J Chem Phys 115(21):9657–9666
24. Liu YH, Neyts E, Bogaerts A (2006) Monte Carlo method for
simulations of adsorbed atom diffusion on a surface. Diam Relat
Mater 15(10):1629–1635
25. Voter A, Montalenti F, Germann T (2002) Extending the time
scale in atomistic simulation of materials. Ann Rev Mater Res
32:321–346
26. Jonsson H, Mills G, Jacobsen KW (1998) Nudged elastic band
method for ﬁnding minimum energy paths of transitions. In:
Berne BJ, Ciccotti G, Coker DF (ed) Classical and quantum
dynamics in condensed phase simulations. World Scientiﬁc,
Singapore
27. Henkelman G, Jonsson H (1999) A dimer method for ﬁnding
saddle points on high dimensional potential surfaces using only
ﬁrst derivatives. J Chem Phys 111:7010–7022
Reprinted from the journal
28. Dellago C, Bolhuis PG, Csajka FS, Chandler D (1998) Transition
path sampling and the calculation of rate constants. J Chem Phys
108(5):1964–1977
29. Barkema GT, Mousseau N (1996) Event-based relaxation of
continuous disordered systems. Phys Rev Lett 77(21): 4358–4361
30. Allen RJ, Warren PB, ten Wolde PR (2005) Sampling rare
switching events in biochemical networks. Phys Rev Lett 94:
018104
31. Ren WE, Vanden-Eijnden E (2005) Finite temperature string
method for the study of rare events. J Phys Chem B 109:6668
32. Faradijan AK, Elber R (2004) Computing time scales from
reaction coordinates by milestoning. J Chem Phys 120:10880–
10889
33. Tironi IG, van Gunsteren WF (1994) A molecular-dynamics
simulation study of chloroform. Mol Phys 83(2): 381–403
34. Laio A, Parrinello M (2002) Escaping free-energy minima. Proc
Natl Acad Sci USA 99(20):12562–12566
35. Zwanzig RW (1954) High temperature equation of state by a
perturbation method. I. Nonpolar gases. J Chem Phys 22:1420–
1426
36. Torrie GM, Valleau JP (1977) Nonphysical sampling distributions in Monte Carlo free-energy estimation: umbrella sampling.
J Comput Phys 22(2):187–199
37. Darve E, Pohorille A (2001) Calculating free energies using
average force. J Chem Phys 115: 9169–9183
38. Leech J, Prins J, Hermans J (1996) SMD: Visual steering of
molecular dynamics for protein design. IEEE Comput Sci Eng
3:38–45
39. Sorensen M, Voter A (2000) Temperature-accelerated dynamics
for simulation of infrequent events. J Chem Phys 112(21):
9599–9606
40. Voter A (1997) Hyperdynamics: accelerated molecular dynamics
of infrequent events. Phys Rev Lett 78(20):3908–3911
41. Voter A (1998) Parallel replica method for dynamics of infrequent events. Phys Rev B Condens Matter 57(22): 13985–13988
42. Egelhoff WF, Jacob I (1998) Reﬂection high-energy electrondiffraction (RHEED) oscillations at 77 K. Phys Rev Lett 62(8):
921–924
43. Georgieva V, Voter AF, Bogaerts A (2011) Understanding the
surface diffusion processes during magnetron sputter-deposition
of complex oxide Mg-Al-O thin ﬁlms. Cryst Growth Des 11(6):
2553–2558
44. Fichthorn KA, Miron RA, Wang YS, Tiwary Y (2009) Accelerated molecular dynamics simulation of thin-ﬁlm growth with the
bond-boost method. J Phys Condens Matter 21(8):084212
45. Hamelberg D, Mongan J, McCammon JA (2004) Accelerated
molecular dynamics: a promising and efﬁcient simulation method
for biomolecules. J Chem Phys 120(24): 11919–11929
46. Uberuaga BP, Stuart SJ, Windl W, Masquelier MP, Voter AF
(2012) Fullerene and graphene formation from carbon nanotube
fragments. Comput Theor Chem 987(SI):115–121
47. Mees MJ, Pourtois G, Neyts EC, Thijsse BJ, Stesmans A (2012)
Uniform-acceptance force-bias Monte Carlo method with time
scale to study solid-state diffusion. Phys Rev B 85(13):134301
48. Laberge L, Tully J (2000) A rigorous procedure for combining
molecular dynamics and Monte Carlo simulation algorithms.
Chem Phys 260(1-2):183–191
49. Ribeiro AAST, de Alencastro RB (2012) Mixed Monte Carlo/
molecular dynamics simulations in explicit solvent. J Comput
Chem 33(8):901–905
50. Ulmschneider JP, Jorgensen WL (2003) Monte Carlo backbone
sampling for polypeptides with variable bond angles and dihedral
angles using concerted rotations and a Gaussian bias. J Chem
Phys 118(9):4261–4271
51. Leach AR (2001) Molecular modelling: principles and applications. Prentice Hall, Essex
287
123
Theor Chem Acc (2013) 132:1320
52. Bussi G, Donadio D, Parrinello M (2007) Canonical sampling
through velocity rescaling. J Chem Phys 126(1):014101
53. Forray C, Muthukumar M (2006) Langevin dynamics simulations
of genome packing in bacteriophage. Biophys J 91:25–41
54. Duane S, Kennedy A, Pendleton B, Roweth D (1987) Hybrid
Monte-Carlo. Phys Lett B 195(2):216–222
55. Mehlig B, Heermann D, Forrest B (1992) Hybrid Monte-Carlo
method for condensed-matter systems. Phys Rev B 45(2):
679–685
56. Clamp ME, Baker PG, Stirling CJ, Brass A (1994) Hybrid MonteCarlo—an efﬁcient algorithm for condensed matter simulation.
J Comput Chem 15(8):838–846
57. Brotz FA, Depablo JJ (1994) Hybrid Monte-Carlo simulation of
silica. Chem Eng Sci 49(17):3015–3031
58. Pangali C, Rao M, Berne B (1978) Novel Monte-Carlo scheme
for simulating water and aqueous-solutions. Chem Phys Lett
55(3):413–417
59. Rao M, Pangali C, Berne B (1979) Force bias Monte-Carlo
simulation of water—methodology, optimization and comparison
with molecular-dynamics. Mol Phys 37(6):1773–1798
60. Dereli G (1992) Stillinger-Weber type potentials in Monte-Carlo
simulation of amorphous-silicon. Mol Simul 8(6):351–360
61. Mezei M (1991) Distance-scaled force biased Monte Carlo simulation for solutions containing a strongly interacting solute. Mol
Simul 5:405–408
62. Timonova M, Groenewegen J, Thijsse BJ (2010) Modeling diffusion and phase transitions by a uniform-acceptance force-bias
Monte Carlo method. Phys Rev B 81(14):144107
63. Neyts EC, Thijsse BJ, Mees MJ, Bal KM, Pourtois G (2012)
Establishing uniform acceptance in force biased Monte Carlo
simulations. J Chem Theory Comput 8: 1865–1869
64. Rossky P, Doll J, Friedman H (1978) Brownian dynamics as
smart Monte-Carlo simulation. J Chem Phys 69(10): 4628–4633
65. Chiu S, Jakobsson E, Scott H (2001) Combined Monte Carlo and
molecular dynamics simulation of hydrated lipid-cholesterol lipid
bilayers at low cholesterol concentration. Biophys J 80(3):
1104–1114
66. Chiu S, Jakobsson E, Subramaniam S, Scott H (1999) Combined
Monte Carlo and molecular dynamics simulation of fully
hydrated dioleyl and palmitoyl-oleyl phosphatidylcholine lipid
bilayers. Biophys J 77(5):2462–2469
67. Jager HU, Belov AY (2003) ta-C deposition simulations: ﬁlm
properties and time-resolved dynamics of ﬁlm formation. Phys
Rev B 68(2):024201
68. Taguchi M, Hamaguchi S (2006) Molecular dynamics study on
Ar ion bombardment effects in amorphous Sio2 deposition processes. J Appl Phys 100(12):123305
69. Taguchi M, Hamaguchi S (2007) Md simulations of amorphous
Sio2 thin ﬁlm formation in reactive sputtering deposition processes. Thin Solid Films 515(12):4879–4882
70. Tavazza F, Nurminen L, Landau D, Kuronen A, Kaski K (2004)
Hybrid Monte Carlo-molecular dynamics algorithm for the study
123
71.
72.
73.
74.
75.
76.
77.
78.
79.
80.
81.
82.
83.
84.
288
of islands and step edges on semiconductor surfaces: application
to Si/Si(001). Phys Rev E 70(3, Part 2): 036701
Tiwary P, van de Walle A (2011) Hybrid deterministic and stochastic approach for efﬁcient atomistic simulations at long time
scales. Phys Rev B 84(10):100301
Grein C, Benedek R, Delarubia T (1996) Epitaxial growth simulation employing a combined molecular dynamics and Monte
Carlo approach. Comput Mater Sci 6(2):123–126
Eckert M, Mortet V, Zhang L, Neyts E, Verbeeck J, Haenen K,
Bogaerts A (2011) Theoretical investigation of grain size tuning
during prolonged bias-enhanced nucleation. Chem Mater 23(6):
1414–1423
Eckert M, Neyts E, Bogaerts A (2009) Modeling adatom surface
processes during crystal growth: a new implementation of the
metropolis Monte Carlo algorithm. CrystEngComm 11(8):1597–
1608
Eckert M, Neyts E, Bogaerts A (2010) Insights into the growth of
(ultra) nanocrystalline diamond by combined molecular dynamics
and Monte Carlo simulations. Cryst Growth Design 10(7):
3005–3021
Neyts EC, Khalilov U, Pourtois G, Van Duin ACT (2011)
Hyperthermal oxygen interacting with silicon surfaces: adsorption, implantation, and damage creation. J Phys Chem C 115(11):
4818–4823
Buffat P, Borel J (1976) Size effect on melting temperature of
gold particles. Phys Rev A 13(6):2287–2298
Jiang A, Awasthi N, Kolmogorov AN, Setyawan W, Borjesson A,
Bolton K, Harutyunyan AR, Curtarolo S (2007) Theoretical study
of the thermal behavior of free and alumina-supported Fe-C
nanoparticles. Phys Rev B 75(20):205426
Shibuta Y, Suzuki T (2010) Melting and solidiﬁcation point of
fcc-metal nanoparticles with respect to particle size: a molecular
dynamics study. Chem Phys Lett 498(4–6): 323–327
Neyts EC, Shibuta Y, Van Duin ACT, Bogaerts A (2010) Catalyzed growth of carbon nanotube with deﬁnable chirality by
hybrid molecular dynamics-force biased Monte Carlo simulations. ACS Nano 4(11): 6665–6672
Neyts EC, Van Duin ACT, Bogaerts A (2011) Changing chirality
during single-walled carbon nanotube growth: a reactive molecular dynamics/Monte Carlo study. J Am Chem Soc 133(43):
17225–17231
Neyts EC, Van Duin ACT, Bogaerts A (2012) Insights in the
plasma-assisted growth of carbon nanotubes through atomic scale
simulations: effect of electric ﬁeld. J Am Chem Soc 134(2):
1256–1260
Hatakeyama R, Kaneko T, Kato T, Li YF (2011) Plasma-synthesized single-walled carbon nanotubes and their applications.
J Phys D Appl Phys 44(17):174004
Kato T, Hatakeyama R (2006) Formation of freestanding singlewalled carbon nanotubes by plasma-enhanced CVD. Chem Vap
Depos 12(6):345–352
Reprinted from the journal